c

Owned by the authors, published by EDP Sciences, 2012

**Coupling of plasticity and damage in glass fibre reinforced polymer**

**composites**

### R. Kvale Joki

1,2,a_{, F. Grytten}

1_{, and H. Osnes}

2
1_{SINTEF Materials & Chemistry}

2_{University of Oslo, Applied Mathematics and Mechanics}

**Abstract.** This study addresses the nonlinear stress-strain response in glass fibre reinforced polymer composite laminates.
Loading and unloading of these laminates indicate that the nonlinear response is caused by both damage and plasticity. A user
defined material model is implemented in the finite element code LS-DYNA. The damage evolution is based on the Puck failure
criterion [1], and the plastic behaviour is based on the quadratic Hill yield criterion for anisotropic materials [2].

**1 Introduction**

A major challenge in composite design is to calculate the damage state and the residual strength after failure initiation. Composite materials have been thought to be brittle with little or no ability for plastic deformation [1]. Non-linear stress-strain response has therefore been treated as damage. Here damage refers to the more or less gradual developments of micro cracks in the matrix material which lead to macro cracks and then finally to ultimate failure caused by fibre failure.

In experiments conducted on laminated glass fibre reinforced polymer composites (GFRPCs) it has been shown that when the specimens were unloaded after tensile loading, irreversible strains had emerged. This indicates that non-linearity is not only caused by damage, but also by plasticity. When loaded a second time, the stress-strain curve also showed some hysteresis, indicating visco-elastic behaviour of the composites.

It is known that composite materials are sensitive to impact loading. A key aspect of an impact event is the impact energy. If one is to understand how the impact energy is absorbed, it is crucial to understand the material response. A non-linear stress-strain response caused by elastic-plastic deformation with irreversible strains ab-sorbs more energy than the equivalent response caused by elastic-damage deformation without irreversible strains, since the dissipated energy equals the area circumfered by the stress-strain curve, see Figure 2 and 3. A presence of hysteresis in the cyclic loading may also serve to dissipate some amount of energy if the propagation of shock waves trough the material causes a large number of oscillations in the local state of stress.

To evaluate the damage progression a material model
based on the Puck failure criterion has been implemented
in the LS-DYNA finite element code. The Puck criterion
[1] was ranked as one of the most promising in the
World Wide Failure Exercises (WWFE) [4]. One of the
conclusion from the WWFE was that the criteria should
treat fibre failure and matrix failure separately. For
pro-gressive failure analysis this is a crucial aspect since fibre
failure and matrix failure evolve quite diﬀerently. The
a_{e-mail:}_{reidar.joki@sintef.no}

Puck criterion diﬀerentiates between Fibre failure (FF) and Inter Fibre failure (IFF). The FF criterion evaluate fibre failure in compression and tension, and the IFF criterion evaluates all failure mechanisms associated with the matrix in compression, tension and shear. The criterion has sepa-rate expressions for tension and compression for both FF and IFF. When the conditions defined by the FF criterion are reached in an integration point, the material model reduces the stiﬀness in that location to zero by deleting the element containing that integration point. When the conditions defined by the IFF criterion are present in an integration point, on the other hand, the material model reduces the stiﬀness in that integration point separately, representing the softening caused by the progression of a smeared damage.

To include plastic strain, the quadratic Hill yield cri-terion has also been implemented in the LS-DYNA fi-nite element code. The quadratic Hill yield criterion for anisotropic materials [2] is an extension the von Mises criterion for isotropic materials, containing six parameters specifying the state of anisotropy. When describing trans-versely isotropic materials, four parameters are suﬃcient.

The evolution of both damage and plasticity is based on the nonlinear response calculated from tensile testing of various laminates. It is assumed that the global nonlinearity is caused by mechanisms in the matrix material alone, and that the fibres behave linearly elastic until sudden failure. The stress-strain curves from standard tensile tests can be replicated by pure damage models as well as pure plastic models, but when the specimens are unloaded after straining the response can not be replicated by damage or plasticity alone. The actual response call for a model based on both damage and plasticity.

The tested laminates are made of standard E-glass
fibres embedded in an epoxy based vinylester matrix1_{.}
The laminates are made of vacuum infused non crimp
fabric. Since the laminates are laid up as non crimp
fabric, the unidirectional laminates have 5% of the fibre
weight fraction in the transverse direction. When modeling
these layers it is assumed that the fibres in the transverse
direction can be evaluated as distinct layers with the same
volume fraction as the fibres in the longitudinal direction.
1_{DION 9102 by Reichold.}

**2 The Puck failure criterion**

The Puck failure criterion is applicable to composite lami-nates built up of unidirectional plies. The plies are assumed to be transversely isotropic and the anisotropy is defined by Cartesian coordinate axes, with 1-direction being in the direction parallel to the fibres, 2-direction being the orthogonal in-plane direction, and the 3-direction the ply normal. The plane of isotropy is defined by the 2- and 3-axes.

**2.1 Fibre failure**

It is assumed that there exists a perfect adhesion between fibre and matrix, i.e. the strain parallel to the fibres (11) are the same for both fibres (f1) and matrix(m1):f1 = 11. Under combined loading the strain in the fibres will be: f1=σf1

*E*f1 −

νf12

*E*f1*m*σfσ22, whereνf12is the Poisson’s ratio for
the fibres, and *m*_{σ}f accounts for the stress magnification
eﬀect2_{caused by the di}_{ﬀ}_{erent moduli of matrix and fibres,}
which leads to an uneven distribution of σ22 from a
microscopic point of view. Thus the longitudinal stress
in the fibres (σf1) under combined loading is defined
as: σf1 = 11*E*f1 + νf12*m*σfσ22. Therefore the failure
condition for fibre failure under combined loading can be
described as:

1
1*T*

11+ νf12

*E*f1

*m*_{σ}fσ2

=1 for (...)1, (1)

were1*T*is the ultimate tensile strain in the longitudinal
di-rection. Experimental results have shown that when a
sig-nificant shear stress,τ12, is superimposed, the compressive
strength is significantly reduced. Puck has therefore added
a shear correction factor to the criterion for compressive
load:

1 1C

11 +νf12

*E*f1

*m*_{σ}fσ22+(10γ21)2=1for(...)<1, (2)

where1*C*is the ultimate compressive strain in the
longitu-dinal direction, and (10γ21)2_{is a purely empirical term. It}
is preferable to use an expression withγ21instead ofτ21,
because the value ofτ21is unknown after failure initiation,
whereas the value ofγ21is not.

**2.2 Inter fibre failure**

The Puck failure criterion has an analytical solution for
in-plane loading and failure conditions [1] (in two
di-mensional analysis). When taking into account out of
plane eﬀects, i.e. trough the thickness shear variations,
and loading conditions in three dimensions, the Puck IFF
criterion has no analytical solution. A full 3-D formulation
of the Puck IFF criterion was used by Wigand et al. [5],
2_{For glass fibre}_{m}

σf≈1.3, and for carbon fibre*m*σf≈1.3 [1].

**Fig. 1.**Illustration of the fracture surface and the stress
compo-nents acting on the surface [1].

and is formulated as:

*e*2=

σn

*R*n
2

+

τn1

*R*n1−*p*n1σn
2

+

τnt

*R*nt−*p*ntσn
2

=1 for σn0,

*e*2=

τn1

*R*n1−*p*n1σn
2

+

τnt

*R*nt−*p*ntσn
2

=1 for σn<0, (3)

where the stress componentsσn,τn1andτntare the stresses
acting on the fracture surface as illustrated in Figure 1
and defined by the angle of the fracture surface, θfp, in
Equation (5). The parameter *R*n describes the resistance
of the fracture plane against normal failure induced by
σn. The parameters*R*n1 and*R*nt are the resistance of the
fracture plane against shear, and finally,*p*n1and*p*ntare the
slope parameters representing internal friction eﬀects [5].
Puck suggests the following values for these parameters [6]

*R*n =*S*+_{22},

*R*n1 =*S*12,

*R*nt =

*S*−_{22}

2 tan(θ0 fp)

,

*p*nt =−
1
tan(2θ0

fp) ,

*p*n1 =*p*nt

*R*n1

*R*nt

. (4)

Here,*Yt*and*Yc*are the transverse strengths in tension and
compression, respectively, and *S*12 is the shear strength.
The angle θ0_{fp} is the angle at which a specimen loaded
in uniaxial compression in the transverse fibre direction
fracture due to shear failure. When subjected to in-plane
loading, IFF is provoked by σ22 and τ12. The shape of
the failure envelope depends strongly onθ0

surface, and are calculated as:

σn =σ22cos2θfp+σ33sin2θfp

+2σ23cosθfpsinθfp, τn1 =σ12cosθfp+σ13sin2θfp,

τnt =−σ22sinθfpcosθfp+σ33sinθfpcosθfp

+σ23(cos2_{θfp}_{−}_{sin}2_{θfp).} _{(5)}
Because no analytical solution to the criterion is possible,
one needs to search through all the possible failure surfaces
to find the one in where the criterion has its maximum
value. The criterion is defined by the failure surface stress
componentsσn,τn1andτnt, and consequently they have to
be calculated for every search angle. Because of symmetry,
the search for the action plane can be limited to the
range−90◦ θ 90◦. A cost eﬀective methodology is
the Golden Section Search [5]. This procedure has been
proven to be an eﬀective tool when searching for the action
plane using the Puck criterion by Wiegand et al. [5].

The strength parameters found in the IFF criterion
(*S*+_{22},*S*−_{22}and*S*12) represents the end of the linearity in the
stress-strain response. The reasons for this non-linearity
are plastic and viscoelastic behaviour of the matrix and,
probably above all, micro-damage [7]. Typically a micro
crack in the matrix propagate until it is stopped by a
crossing fibre. At the location of the micro-damage, the
stiﬀness of the matrix is reduced to zero, while the rest of
the matrix material holds the initial stiﬀness. As more and
more of these micro cracks develops, the overall global
stiﬀness will be degraded in a progressive manner. The
development of these micro-cracks will aﬀect the global
transverse stiﬀnesses*E*22and*E*33, the in- and out-of-plane
shear stiﬀness’s*G*12 and*G*13, the transverse out-of-plane
shear stiﬀness *G*23, the in- and out-oﬀ-plane Poisson’s
ratioν12andν13and the transverse out-oﬀ-plane Poisson’s
ratio ν23. It is reasonable to address the development of
micro-damage as smeared, and degrade the*E*22,*E*33,*G*12,

*G*13,ν12,ν13 andν23 with a progressive reduction factor.
In [7], Puck argues that these material properties may be
reduced concurrently by the same reduction factor,η. Puck
also argues that the following expression is a reasonable
approach to this reduction factor [7]:

η= 1−ηr

1+*c*(*f*E(IFF)−1)ξ

+ηr, (6)

where the dimensionless parameters*c*andξserve to fit the
η-curve to experimental results. The termη*r* represents a
small remaining stiﬀness (ηr <1). The values of*c*,ξandηr
has been determined using the optimization code LS-OPT.
The simulated response has been fitted to experimental
results from tensile loading of 6-layered laminates with 5%
of the fibres in each layer in the longitudinal direction and
95% in the transverse direction. It is assumed that the 5%
of the fibres that are oriented in the longitudinal direction
behave elastic untill failure.

Figure 2 illustrates the on and oﬀloading response of a [±45]6-laminate when nonlinearity is caused by damage alone. The laminate is loaded and unloaded at point 1, 2 and 3. The unloading follows a linear-elastic path to zero stress and strain. When the laminate is resloaded, the

**Fig. 2.** Three cycles of loading and unloading of [±45]6
-laminates.

stress-strain curve follows the same path as when unloaded until it succeedes the stress level of the previous unloaded. As the stress level is increased, further damage is induced by continued reduction of the secant stiﬀness.

**3 The Hill yield criterion**

The original Hill yield criterion [2] has a quadratic form, and is a straightforward extension of the von Mises yield criterion. It is defined by three axes of anisotropy.

¯

σ2_{=}_{F}_{(σ22}_{−}_{σ33}_{)}2 _{+}_{G}_{(σ33}_{−}_{σ11}_{)}2

+*F*(σ11−σ22)2+2*L*σ2_{23}

+2*M*σ2_{31} +2*N*σ2_{12}. (7)
Here *F, G, H, L, M* and *N* are constants that have to
be determined experimentally, σ*i j* are the stresses with
reference to the axes of anisotropy and ¯σis the eﬀective
stress. For composite laminates made up of unidirectional
plies, the axes of anisotropy are orthogonal. The constants
can be determined from [2]:

*F*= 1

2
σ0
σy_{22}

2

+

σ0

*S*y_{33}

2

−

σ0

*S*_{11}y

2 ,

*G*= 1

2 σ0

*S*y_{33}

2

+

σ0

*S*y_{11}

2

−

σ0

*S*y_{22}

2 ,

*H*= 1

2 σ0

*S*y_{11}

2

+

σ0

*S*_{22}y

2

− σ0

*S*y_{33}

2

(8)

and

*L*= 1

2 σ0

*S*y_{23}

2

,

*M* = 1

2 σ0

*S*y_{31}

2

,

*N*= 1

2

σ0

*S*y_{12}

2 ,

(9) where σ0 is the eﬀective stress at initiation of plasticity.

**Fig. 3.** Three cycles of loading and unloading of the [±45]6
-laminates.

As mentioned above, it is assumed that the plane
orthogonal to the fibre direction is isotropic. By this
assumption of transverse isotropy it follows that*S*22 =*S*33
and*S*12 =*S*13, which again serves to reduce the number
of constants from six to four, i.e.*G* = *H* and *M* = *N*.
Therefore the quadratic Hill yield criterion can be reduced
to:

¯

σ2 _{=}_{F}_{(σ22}_{−}_{σ33)}2

+*G*(σ33−σ11)2+(σ11−σ22)2

+2*L*σ2_{23}+2*M*σ2_{13} +σ2_{12}. (10)
Figure 3 illustrates the on and oﬀ loading response
of a [±45]6-laminate when nonlinearity is assumed to be
caused by plasticity alone. The laminate is loaded and
unloaded at the same strain levels as the laminate described
in 2, at 1, 2 and 5% strain. When the nonlinearity is
described by plasticity, the nonlinearity is achieved by
introducing irreversible strains. This is evident when the
laminate is unloaded and the stress level is reduced to
zero, the strain level is non-zero. It can be seen that the
on and oﬀloading paths 1-2, 3-4 and 5-6, have the same
gradient, indicating that the global stiﬀness of the laminate
is preserved.

**4 Material tests**

All the material properties used to describe the elastic be-haviour are based on an extensive material testing exercise using low strain rates. The tensile tests are carried out in accordance to the ASTM D3039 standard, the compressive tests, to the ASTM D6641 and the shear properties are obtained from ASTM D 3518 and ASTM D7078. Seven diﬀerent laminate lay-ups have been tested [0]6, [90]6, [0/90]6, [±45]6, [0/45/90/−45]6, [±45/(0)6/±45] and [±45/(90)6/±45], where the numbers within the brackets indicate the orientation of the longitudinal ply direction with respect to the loading direction, the order of the num-bers indicate the stacking sequence and the subscript out side the brackets, how many times the sequence is repeated through the laminate. The deduced elastic material proper-ties are displayed in Table 1 and the strength parameters (with respect to damage) are displayed in Table 2. The parameters needed to evaluate the Puck failure criterion are displayed in Table 3, here the fracture angle for pure transverse compression,θfp, is obtained from literature for

**Table 1.**Elastic material properties.

*E11* 42028 MPa

*E22* 11472 MPa

*G12* 4000 MPa

ν12 0.25

ν23 0.30

**Table 2.**Material strength.

*S*_{11}+ 1100 MPa

*S*_{22}+ 28 MPa

*S*_{11}− 600 MPa

*S*_{22}− 200 MPa

*S12* 50 MPa

*S23* 50 MPa

**Table 3.**Properties for the Puck criterion.

θ0
*f p* 51
*E*+_{1}* _{f}* 73000 MPa

ν1*f* 0.20

**Table 4.**Properties for the Hill criterion.

*F* 0.9997

*G* 3.24E-05

*L* 0.160

*M* 0.160

an equivalent material. The plasticity parameters needed to evaluate the Hill criterion are calculated as described above, and displayed in Table 4.

Two sets of laminates have been subjected to cycles of loading and unloading, namely [0/90]6- and [±45]6 -laminates. The strain rate and on- and oﬀ-loading tests has been conducted using the setup and test specimen geome-try from the ASTM D 3039 test standard. The results are presented in Figure 4 and 5. It is assumed that the lon-gitudinally oriented plies in the [0/90]6-laminates behave elastically within the 2.5% strain. This assumption is based on an evaluation of the stress-strain curves produced from tensile tests on the various laminates mentioned above. Therefore the nonlinearity is thought to be caused by mechanisms in the transversely oriented plies. In Figure 6 the response from the transversely oriented plies has been isolated using classical laminate theory (the Poisson eﬀects are disregarded).

**Fig. 4.**Three cycles of loading and unloading of the [±45]6
-laminates.

**Fig. 5.**Three cycles of loading and unloading of the [0/90]6
-laminates.

**Fig. 6.**The response in the transversely oriented plies from three
cycles of loading and unloading of the [0/90]6-laminates.

damage, indicated by the severe reduction in secant stiﬀ -ness in each unloading.

**5 Coupling of yield and damage**

In the material test results presented in Figure 4, 5 and 6, both irreversible strains and reduction in secant stiﬀness is observed. Irreversible strains are commonly associated with plasticity and reduction in secant stiﬀness, with dam-age.

It is assumed that the longitudinal response is linear up to ultimate failure, the nonlinear shear response is caused by plasticity and that the nonlinear transverse tensile response is caused by damage. The failure criterion was adjusted not to aﬀect any of the shear moduli, i.e.

*G*12,*G*13 and *G*23. The yield criterion was adjusted not

**Fig. 7.**Stress-strain curves from tensile loading experiments and
simulation of [90]6-laminates.

**Fig. 8.**Stress-strain curves from tensile loading experiments and
simulation of [0]6-laminates.

**Fig. 9.**Stress-strain curves from tensile loading experiments and
simulation of [0/90]6-laminates. The simulation is unloaded and
reloaded 1%, 3% and 5% strain.

to aﬀect the response in the transverse direction or in the longitudinal direction, and also, the shear response was assumed to be isotropic. The hardening curve was established based on the shear response of the ASTM D 3518 test on [±45]6-laminates.

**6 Simulation results**

**Fig. 10.**Stress-strain curves from tensile loading experiments and
simulation of [0/±45]6-laminates.

**Fig. 11.**Stress-strain curves from tensile loading experiments and
simulation of [±45]6-laminates. The simulation is unloaded and
reloaded 1.5% and 2% strain.

**7 Discussion**

It has been shown that the presented model gives a good estimation of the nonlinear response these laminates have to tensile loading. The cyclic loading results form the simulations are in good agreement with that observed in the experimental results. This model will be further refined for use in impact modeling. In an impact-event, elastic stress waves will cause local stress oscillations which will contribute to dissipate the impact energy. When predicting the residual strength after impact, it is crucial to have a good understanding of the mechanisms involved in the dissipation of the impact energy.

**Fig. 12.**Stress-strain curves from tensile loading experiments and
simulation of [0/45/90/−45]6-laminates.

**Acknowledgements**

This work is part of the project *“Composite structures under*
*impact loading”* financed by the Norwegian Reserch Council
(193238/i40), Flowtite Technology AS, Nammo Raufoss AS and
Ragasco AS. The authors would like to express their thanks for
this finacial support. The authors would also like to thank the
other partners in the project (NTNU, UiO and SINTEF Raufoss
Manufacturing) for constructive discussions.

**References**

1. A. Puck and H. Sch¨urmann, Composites Science and
Technology**58**, (1998) 1045-1067

2. R. Hill, Proceedings of the Royal Society of London.
Series A, Mathematical and Physical Sciences **193**,
(1948) 281-297

3. X. Xiao, A Coupled Damage-plasticity Model for En-ergy Absorption in Composites

4. M.J. Hinton, A.S. Kaddour and P.D. Soden, *Failure*
*criteria in Fibre reinforced polymer composites: The*
*World-Wide Failure Exercise*(Elisvier, 2003) 1255
5. J Wiegand, N Petrinic and B Elliott, Composites

Sci-ence and Technology**68**, (2008) 2511-2517

6. A. Puck, J. Kopp and M. Knops, Composites Science
and Technology**62**, (2002) 371-378